MANUFACTURING GUIDE

BioMed White ResinEN

Manufacturing Guide

DE

Fertigungsleitfaden

FR

Guide de fabrication

IT

Guida alla produzioneES

Guía de fabricaciónKO제조 가이드

JA

マニュファクチャリングガイド

ZH

制造指南

Prepared: 02/29/2024 PRNT-0104 Rev 02

Specific Manufacturing Considerations
The BioMed White Resin specifications have been validated using the hardware and parametersindicated below. For biocompatibility compliance, validation used a dedicated resin tank and mixer,
build platform, wash unit and post-processing equipment that were not mixed with any other resins.

1. Hardware:a. Formlabs 3D Printer: Form 2, Form 3B/3B+, Form 3BL, Form 4B
b. Print Accessories: Formlabs Build Platforms, Formlabs Resin Tanks

2. Software:a. Formlabs Preform

3. Printing Parameters:a. Layer Thickness: 100 μm and 50 μm

4. Recommended Post-Processing Equipment and Accessories:
a. Formlabs Processing Accessories: Form Auto, Resin Pumping Systemb. Formlabs Validated Wash Unit: Form Wash, Form Wash (2nd Generation), Form Wash L, Ultrasonic
Wash Unitc. Formlabs Validated Cure Unit: Form Cure, Form Cure L, Fast CureA. PRINTING
1. Shake cartridge: Shake the cartridge before every print job. Color deviations and print failures
may occur if the cartridge is shaken insufficiently.
2. Set up: Insert resin cartridge into a compatible Formlabs 3D printer. Insert resin tank and attach
mixer to the tank.
3. Printing:a. Prepare a print job using PreForm software. Import desired part STL file.
b. Orient and generate supports.
c. Send the print job to the printer.
d. Begin print by selecting a print job from the print menu. Follow any prompts or dialogs shownon the printer screen. Printer will automatically complete the print.

B. PART REMOVAL
Remove the build platform from the printer. To remove parts from the build platform, wedge the part
removal tool under the printed part raft, and rotate the tool. Formlabs Build Platform 2 or Build Platform
2L may be used for easy, tool free removal. For detailed techniques visit support.formlabs.com.

C. WASHING
Place the printed parts in a Formlabs-validated wash unit with 99% Isopropyl Alcohol.
1. Form Wash, Form Wash (2nd Generation) - High speed*, or Form Wash L:a. Wash for 5 minutes or until clean.
b. If parts do not appear clean after washing, consider replacing used Isopropyl Alcohol in thewash unit with fresh solvent.
*For Form Wash (2nd Gen), High speed settings are validated for use.
2. Ultrasonic Wash Unit:
NOTE: Using Isopropyl Alcohol in an ultrasonic bath presents a risk of fire or explosion. When using
an ultrasonic wash read and follow all safety recommendations from the ultrasonic wash manufacturer.
a. Use clean 99% Isopropyl Alcohol for each wash.
b. Place parts in a secondary disposable plastic container or plastic resealable bag then fill with
99% Isopropyl Alcohol, ensuring parts are fully submerged.

ENGLISH

BioMed White Resin is a light-curable, polymerizable resin material for the additive manufacturingof biocompatible, medical grade, white parts that are robust and extremely versatile. Users should
independently verify the suitability of the printed materials for their particular application andintended purpose. This Manufacturing Guide will give equipment, printing and post-processing
recommendations and requirements to ensure the correct and safe usage of this material.

c. Place the secondary container in the ultrasonic unit water bath and sonicate for 2 minutes oruntil clean.**Washing efficacy depends on the ultrasonic unit size and power. Formlabs testing was conductedwith ultrasonic units at 36 W/L or higher.

D. DRYING
1. Remove parts from Isopropyl Alcohol and leave to air dry at room temperature for at least 30 minutes.
NOTE: Dry times can vary depending on the design of parts and ambient conditions. Do not letparts sit in Isopropyl Alcohol for longer than needed.
2. Inspect printed parts to ensure that parts are clean and dry. No residual solvent, excess liquid resinor residue particles should remain on the surface before proceeding to subsequent steps.
3. If the residual solvent is still present, dry parts longer. If resin residue is still visible, rewash parts
until clean and dry.

E. POST-CURING
Place the printed parts in a Formlabs-validated post-curing unit and cure for the required time.
1. Form Cure or Form Cure L:
a. Cure for 60 minutes at 60 °C
b. Allow the Form Cure or Form Cure L unit to cool down to room temperature between cure
cycles.
2. Fast Cure:a. Cure for 6 minutes at Light Intensity 5b. Allow the Fast Cure unit to cool for at least 10 minutes between cure cycles.

F. SUPPORT REMOVAL & POLISHING
1. Remove supports using a cutting plier, cutting disk and a handpiece, or by using other part
removal tools. If needed, rough marks left on the surface of the parts after support removal may bepolished/sanded down smooth to improve surface finish.
2. Inspect the parts for any cracks. Discard if any damage or cracks are detected.

G. CLEANING & DISINFECTION
1. The parts may be cleaned, disinfected, and sterilized according to facility protocols. The manufacturer
is responsible for validation of part performance depending on the application requirements post
disinfection and/or sterilization. NOTE: If alcohol-based disinfectants are used, do not leave parts inalcohol solution for an extended time.
2. After cleaning and disinfection inspect the part for damage or cracks to ensure that the integrity ofthe designed part meets performance requirements. Discard if any damage or cracks are detected.

H. HAZARDS, STORAGE & DISPOSAL
1. Cured resin is non-hazardous and may be disposed of as regular waste.
2. See SDS for more information at support.formlabs.com.

Spezifische Überlegungen zur Fertigung
Die Spezifikationen von BioMed White Resin wurden unter Verwendung der unten angegebenen
Hardware und Parameter validiert. Um die Biokompatibilität zu gewährleisten, wurde für die
Validierung ein dedizierter Harztank mit Mischer, eine dedizierte Konstruktionsplattform undWascheinheit sowie dedizierte Nachbearbeitungsgeräte genutzt, die nicht mit anderen Harzen in
Kontakt gekommen sind.

1. Hardware:a. Formlabs-3D-Drucker: Form 2, Form 3B/3B+, Form 3BL, Form 4B
b. Druck-Zubehör: Formlabs Konstruktionsplattformen, Formlabs Harztanks

2. Software:a. Formlabs PreForm

3. Druckparameter:a. Schichtdicke: 100 μm und 50 μm

4. Empfohlene Nachbearbeitungsgeräte und Zubehör:
a. Formlabs-Bearbeitungszubehör: Form Auto, Resin Pumping System
b. Von Formlabs validierte Wascheinheit: Form Wash, Form Wash (2. Generation), Form Wash L,
Ultraschall-Waschgerät
c. Von Formlabs validierte Aushärteeinheit: Form Cure, Form Cure L, Fast Cure

A. DRUCKEN
1. Kartusche schütteln: Schütteln Sie die Kartusche vor jedem Druckauftrag. Wenn die Kartusche
nicht ausreichend geschüttelt wird, können Farbabweichungen und Fehldrucke auftreten.
2. Einrichtung: Setzen Sie die Harzkartusche in einen kompatiblen Formlabs-3D-Drucker ein.
Setzen Sie den Harztank ein und befestigen Sie den Mischer am Tank.
3. Druck:a. Bereiten Sie einen Druckauftrag mit der Software PreForm vor. Importieren Sie die STL-Datei
des gewünschten Teils.
b. Richten Sie das Modell aus und generieren Sie Stützstrukturen.
c. Senden Sie den Druckauftrag an den Drucker.
d. Beginnen Sie den Druckvorgang durch Auswahl eines Druckauftrags aus dem Menü „Print“(Druck). Befolgen Sie alle Aufforderungen oder Dialoge, die auf dem Druckerbildschirmangezeigt werden. Der Drucker schließt den Druckvorgang automatisch ab.

B. ENTFERNEN DER TEILE
Entnehmen Sie die Konstruktionsplattform aus dem Drucker. Um Teile von der Konstruktionsplattform zu
entfernen, klemmen Sie das Ablösewerkzeug unter das Druckteil-Raft und drehen Sie das Werkzeug.
Für ein einfaches, werkzeugloses Entfernen können die Formlabs Build Platform 2 oder die Build
Platform 2L verwendet werden. Detaillierte Techniken finden Sie auf support.formlabs.com.

C. WASCHEN
Legen Sie die Druckteile in ein von Formlabs geprüftes Waschgerät mit 99%igem Isopropylalkohol.
1. Form Wash, Form Wash (2. Generation) - High speed*, oder Form Wash L:a. Waschen Sie die Druckteile 5 Minuten lang oder bis sie sauber sind.
b. Wenn die Teile nach dem Waschen nicht sauber erscheinen, sollten Sie den verwendeten
Isopropylalkohol in der Waschanlage durch frisches Lösungsmittel ersetzen.

DEUTSCH

BioMed White Resin ist ein lichthärtbares, polymerisierbares Harzmaterial für die additive Fertigung
biokompatibler, medizinischer, weißer Teile, die robust und extrem vielseitig sind. Die Eignung desgedruckten Materials für spezifische Anwendungen und Verwendungszwecke sollte vom Nutzer
immer unabhängig überprüft werden. Dieser Fertigungsleitfaden enthält Empfehlungen bezüglich
Geräte, Druck und Nachbearbeitung, damit die korrekte und sichere Verwendung dieses Materials
gewährleistet ist.

*Für Form Wash (2. Generation) sind die Einstellungen für hohe Drehzahl für die Verwendung bestätigt.
2. Ultraschall-Waschgerät:
ANMERKUNG: Bei der Verwendung von Isopropylalkohol in einem Ultraschallbad besteht Brandund Explosionsgefahr. Wenn Sie ein Ultraschallgerät verwenden, lesen und befolgen Sie alle
Sicherheitsempfehlungen des Herstellers des Ultraschallgeräts.
a. Verwenden Sie für jeden Waschvorgang sauberen 99%igen Isopropylalkohol.
b. Platzieren Sie die Teile in einen zweiten Einweg-Plastikbehälter oder einen
wiederverschließbaren Plastikbeutel und füllen Sie ihn mit 99%igem Isopropylalkohol, sodass
die Teile vollständig bedeckt sind.
c. Platzieren Sie den Sekundärbehälter in das Wasserbad des Ultraschallgeräts und beschallen
Sie ihn für 2 Minuten oder bis die Teile sauber sind.**Die Wirksamkeit der Reinigung hängt von der Größe und Leistung des Ultraschallgeräts ab.
Die Formlabs-Tests wurden mit Ultraschallgeräten bei 36 W/L oder höher durchgeführt.

D. TROCKNEN:
1. Nehmen Sie die Teile aus dem Isopropylalkohol und lassen Sie sie mindestens 30 Minuten langbei Raumtemperatur an der Luft trocknen. ANMERKUNG: Die Trockenzeiten können je nach
Teiledesign und Umgebungsbedingungen variieren. Lassen Sie die Teile nicht länger als nötig in
Isopropylalkohol liegen.
2. Untersuchen Sie die Druckteile und stellen Sie sicher, dass sie sauber und trocken sind. Es dürfen
keine Lösungsmittelreste, überschüssiges flüssiges Kunstharz oder Partikelreste auf der Oberfläche
verbleiben, bevor die nachfolgenden Schritte ausgeführt werden.
3. Wenn noch Lösungsmittelreste vorhanden sind, lassen Sie die Teile länger trocknen. Wenn nochHarzreste sichtbar sind, waschen Sie die Teile erneut, bis sie sauber und trocken sind.

E. NACHHÄRTUNG
Platzieren Sie die Druckteile in ein von Formlabs validiertes Nachhärtegerät und lassen Sie sie die
erforderliche Zeit aushärten.
1. Form Cure oder Form Cure L:
a. Aushärtung für 60 Minuten bei 60 °C
b. Lassen Sie das Form-Cure-Gerät oder Form-Cure-L-Gerät zwischen den Aushärtezyklen auf
Raumtemperatur abkühlen.
2. Fast Cure:a. Aushärtung für 6 Minuten bei Lichtintensität 5b. Lassen Sie das Fast-Cure-Gerät zwischen den Aushärtezyklen mindestens 10 Minuten
lang abkühlen.

F. ENTFERNEN DER STÜTZSTRUKTUREN & POLITUR
1. Entfernen Sie die Stützstrukturen mit einer Trennzange, einer Schneidscheibe und einem
Handstück oder mit anderen Ablösewerkzeugen. Falls erforderlich, können raue Stellen auf der
Oberfläche der Teile nach dem Entfernen der Stützstrukturen glatt geschliffen werden, um die
Oberflächengüte zu verbessern.
2. Untersuchen Sie die Teile auf Risse. Entsorgen Sie die Teile, falls Sie Beschädigungen oder
Risse feststellen.

G. REINIGUNG UND DESINFEKTION
1. Die Teile können gemäß den betriebsinternen Anweisungen gereinigt, desinfiziert und sterilisiert
werden. Der Hersteller ist für die Validierung der Leistung des Teils nach der Desinfektion
und/oder Sterilisation gemäß den Anwendungsanforderungen verantwortlich. Hinweis: Wenn
Desinfektionsmittel auf Alkoholbasis verwendet werden, dürfen die Teile nicht für längere Zeit inder Alkohollösung liegen.
2. Prüfen Sie das Teil nach der Reinigung und Desinfektion auf Schäden oder Risse, um sicherzustellen,
dass die Integrität des entworfenen Teils den Leistungsanforderungen entspricht. Entsorgen Sie
die Teile, falls Sie Beschädigungen oder Risse feststellen.

H. GEFAHREN, LAGERUNG UND ENTSORGUNG
1. Ausgehärtetes Harz ist nicht gefährlich und kann als normaler Hausmüll entsorgt werden.
2. Weitere Informationen finden Sie im SDB unter support.formlabs.com.

Considérations particulières relatives à la fabrication
Les spécifications de BioMed White Resin ont été validées en utilisant le matériel et les paramètres
indiqués ci-dessous. Afin d’assurer la biocompatibilité, la validation a utilisé un bac à résine, unmélangeur, une plateforme de fabrication, une unité de lavage et un équipement de post-traitement
dédiés qui n’ont pas été mélangés avec d’autres résines.

1. Matériel :a. Imprimante 3D Formlabs : Form 2, Form 3B/3B+, Form 3BL, Form 4B
b. Accessoires d’impression : plateformes de fabrication Formlabs, bacs à résine Formlabs

2. Logiciel :a. PreForm de Formlabs

3. Paramètres d’impression :a. Épaisseur de couche : 100 μm et 50 μm

4. Équipement et accessoires de post-traitement recommandés :a. Accessoires de traitement Formlabs : Form Auto, Resin Pumping Systemb. Unité de lavage validée par Formlabs : Form Wash, Form Wash (2e génération), Form Wash L,
unité de lavage à ultrasonsc. Unité de polymérisation validée par Formlabs : Form Cure, Form Cure L, Fast Cure

A. IMPRESSION
1. Agitation de la cartouche : secouez la cartouche avant chaque impression. Une agitation
insuffisante de la cartouche peut entraîner des écarts de couleur ou des erreurs d’impression.
2. Installation : insérez la cartouche de résine dans une imprimante 3D Formlabs compatible. Insérez
le bac à résine et fixez le mélangeur au bac.
3. Impression :a. Préparez une tâche d’impression à l’aide du logiciel PreForm. Importez le fichier STL
de la pièce souhaitée.
b. Procédez à l’orientation et générez les supports.
c. Envoyez la tâche d’impression à l’imprimante.
d. Démarrez l’impression en sélectionnant la tâche d’impression dans le menu d’impression.
Suivez toutes les instructions ou boîtes de dialogue affichées sur l’écran de l’imprimante.
L’imprimante va automatiquement effectuer l’impression.

B. RETRAIT DES PIÈCES
Retirez la plateforme de fabrication de l’imprimante. Pour retirer les pièces, calez l’outil pour retirer lespièces de la plateforme sous la base de chaque pièce imprimée et faites tourner l’outil. La Build Platform 2
ou la Build Platform 2L de Formlabs peuvent être utilisées pour un retrait facile et sans outil. Pour destechniques plus détaillées, consultez support.formlabs.com.

C. LAVAGE
Placez les pièces imprimées dans une unité de lavage validée par Formlabs avec de l’alcool
isopropylique à 99 %.
1. Form Wash, Form Wash (2e génération) - Grande vitesse* ou Form Wash L :a. Lavez pendant 5 minutes ou jusqu’à ce que la pièce soit propre.
b. Si les pièces ne semblent pas propres après le lavage, envisagez de remplacer l’alcool
isopropylique usagé dans l’unité de lavage par du solvant propre.

FRANÇAIS

BioMed White Resin est une résine polymérisable photodurcissable pour la fabrication additivede pièces blanches biocompatibles de qualité médicale, robustes et extrêmement polyvalentes.
Les utilisateurs doivent vérifier de manière indépendante si un matériau imprimé convient à leurapplication spécifique et à l’usage auquel il est destiné. Ce guide de fabrication fournit desrecommandations et des exigences en matière d’équipement, d’impression et de post-traitement
afin de garantir une utilisation correcte et sans danger de ce matériau.

*Les paramètres de grande vitesse de la Form Wash (2e génération) sont validés pour l’utilisation.
2. Unité de lavage à ultrasons :REMARQUE : L’utilisation d’alcool isopropylique dans un bain à ultrasons présente un risqued’incendie ou d’explosion. Lors de l’utilisation d’un appareil de lavage à ultrasons, lisez et respectez
toutes les recommandations de sécurité du fabricant de l’appareil.
a. Utilisez de l’alcool isopropylique propre à 99 % pour chaque lavage.
b. Placez les pièces dans un récipient secondaire en plastique jetable ou dans un sac en
plastique refermable, puis remplissez-le d’alcool isopropylique à 99 %, en veillant à ce que lespièces soient entièrement immergées.
c. Placez le récipient secondaire dans le bain de l’unité à ultrasons et effectuez la sonication
pendant 2 minutes ou jusqu’à ce que la pièce soit propre*.
* L’efficacité du lavage dépend de la taille et de la puissance de l’appareil à ultrasons. Les essais deFormlabs ont été réalisés avec des appareils à ultrasons de 36 W/L ou plus.

D. SÉCHAGE
1. Retirez les pièces de l’alcool isopropylique et laissez-les sécher à l’air libre à températureambiante pendant au moins 30 minutes. REMARQUE : Les temps de séchage peuvent varier enfonction du design des pièces et des conditions ambiantes. Ne laissez pas les pièces reposerdans l’alcool isopropylique plus longtemps que nécessaire.
2. Inspectez les pièces imprimées afin de vérifier qu’elles sont bien propres et sèches. Leurs surfaces
doivent impérativement être débarrassées de tout reste de solvant, résine liquide en excès ou
particules résiduelles avant de passer aux étapes suivantes.
3. Si du solvant résiduel est encore présent, faites sécher les pièces plus longtemps. Si des résidus derésine sont encore visibles, lavez à nouveau les pièces jusqu’à ce qu’elles soient propres et sèches.

E. POST-POLYMÉRISATION
Placez les pièces imprimées dans une unité de post-polymérisation validée par Formlabs etpolymérisez-les pendant la durée requise.
1. Form Cure ou Form Cure L :a. Polymérisez les pièces pendant 60 minutes à 60 °C.
b. Laissez la Form Cure ou la Form Cure L refroidir jusqu’à température ambiante entre les cycles
de polymérisation.
2. Fast Cure :a. Polymérisez les pièces pendant 6 minutes à l’intensité lumineuse 5.
b. Laissez la Fast Cure refroidir pendant 10 minutes au minimum entre les cycles de polymérisation.

F. RETRAIT DES SUPPORTS ET POLISSAGE
1. Retirez les supports à l’aide d’une pince coupante, d’un disque de coupe et d’une pièce à main,ou en utilisant d’autres outils pour retirer les pièces de la plateforme. Si nécessaire, les marques
rugueuses laissées sur la surface des pièces après le retrait du support peuvent être polies/
sablées pour améliorer la finition de la surface.
2. Vérifiez que les pièces ne sont pas fissurées. En cas de dommage ou de fissure, jetez-les.

G. NETTOYAGE ET DÉSINFECTION
1. Les pièces peuvent être nettoyées, désinfectées et stérilisées conformément aux protocoles dusite. Le fabricant est responsable de la validation des performances de la pièce en fonction desexigences de l’application après désinfection et/ou stérilisation. REMARQUE : si des désinfectants
à base d’alcool sont utilisés, ne pas laisser les pièces dans la solution alcoolisée pendant une
période prolongée.
2. Après le nettoyage et la désinfection, vérifiez que la pièce n’est pas endommagée ou fissurée afin
de vous assurer que l’intégrité de la pièce conçue répond aux exigences de performance. En cas
de dommage ou de fissure, jetez la pièce.

H. DANGERS, STOCKAGE ET ÉLIMINATION
1. La résine polymérisée n’est pas dangereuse et peut être éliminée avec les déchets ordinaires.
2. Pour plus d’informations, consultez la FDS sur le site support.formlabs.com.

Considerazioni specifiche sulla produzione
Le specifiche della BioMed White Resin sono state convalidate utilizzando l’hardware e i parametriindicati di seguito. Al fine di garantire la conformità alle direttive di biocompatibilità, la convalidaè stata eseguita utilizzando un serbatoio resina, un miscelatore, una piattaforma di stampa, un’unità
di lavaggio e un’attrezzatura di post-elaborazione dedicati, non usati con altre resine.

1. Hardware:a. Stampante 3D Formlabs: Form 2, Form 3B/3B+, Form 3BL, Form 4B
b. Accessori per la stampa: piattaforme di stampa Formlabs, serbatoi resina Formlabs

2. Software:a. PreForm di Formlabs

3. Parametri di stampa:
a. Spessore dello strato: 100 μm e 50 μm

4. Attrezzatura e accessori raccomandati per la post-elaborazione:a. Accessori di lavorazione Formlabs: Form Auto, Resin Pumping Systemb. Unità di lavaggio convalidata Formlabs: Form Wash, Form Wash (seconda generazione),
Form Wash L, unità di lavaggio a ultrasuonic. Unità di polimerizzazione convalidata Formlabs: Form Cure, Form Cure L, Fast Cure

A. STAMPA
1. Agitazione della cartuccia: agita la cartuccia prima di ogni lavoro di stampa. Nel caso in cui la cartuccia
non sia stata agitata a sufficienza potrebbero verificarsi variazioni cromatiche ed errori di stampa.
2. Impostazione: inserisci la cartuccia di resina in una stampante 3D Formlabs compatibile. Inserisci
il serbatoio resina e collega il miscelatore al serbatoio.
3. Stampa:
a. Prepara un lavoro di stampa utilizzando il software PreForm. Importa il file STL dellaparte desiderata.
b. Orienta e genera i supporti.
c. Invia il lavoro di stampa alla stampante.
d. Avvia la stampa selezionando il lavoro di stampa dall’apposito menu. Segui le istruzionio le finestre di dialogo visualizzate sullo schermo della stampante. La stampante completerà
la stampa in modo automatico.

B. RIMOZIONE DELLE PARTI
Rimuovi la piattaforma di stampa dalla stampante. Per rimuovere le parti, inserisci l’apposito strumento
sotto la base della parte stampata e ruotalo. Usa la Build Platform 2 o la Build Platform 2L di Formlabs
per una rimozione semplice e senza strumenti. Per tecniche dettagliate, visita support.formlabs.com.

C. LAVAGGIO
Posiziona le parti stampate in un’unità di lavaggio convalidata da Formlabs con alcool isopropilico al 99%.
1. Form Wash, Form Wash (seconda generazione)* o Form Wash L:
a. Lavale per cinque minuti o finché non sono pulite.
b. Se le parti non risultano pulite dopo il lavaggio, sostituisci l’alcool isopropilico con solvente pulito.
*Per la Form Wash (seconda generazione), le impostazioni di alta velocità sono convalidate per l’uso.
2. Unità di lavaggio a ultrasuoni:
NOTA: l’utilizzo di alcool isopropilico in un bagno a ultrasuoni presenta un rischio di incendio oesplosione. Quando utilizzi un lavaggio a ultrasuoni, leggi e segui tutte le disposizioni di sicurezza
fornite dall’azienda produttrice.

ITALIANOLa BioMed White Resin è un materiale in resina fotopolimerizzabile per la produzione additiva di parti
biocompatibili di colore bianco adatte all’uso medico, robuste ed estremamente versatili. Spetta agli
utenti verificare autonomamente l’idoneità del materiale stampato per l’impiego e lo scopo previsti.
Consulta questa guida alla produzione per conoscere le raccomandazioni e i requisiti in merito astampa, post-elaborazione e apparecchi, al fine di garantire l’uso corretto e sicuro di questo materiale.

a. Utilizza alcool isopropilico al 99% pulito in ogni lavaggio.
b. Posiziona le parti in un contenitore in plastica monouso secondario o in un sacchetto diplastica richiudibile, quindi versa alcool isopropilico al 99% assicurandoti che le parti sianocompletamente immerse.
c. Posiziona il contenitore secondario nel bagno d’acqua dell’unità a ultrasuoni e applica gli
ultrasuoni per due minuti o finché le parti non sono pulite.**L’efficacia del lavaggio dipende dalle dimensioni e dalla potenza dell’unità a ultrasuoni. I test
di Formlabs sono stati condotti con unità a ultrasuoni a una potenza di 36 W/L o superiore.

D. ASCIUGATURA
1. Rimuovi le parti dall’alcool isopropilico e lasciale asciugare a temperatura ambiente per almeno
30 minuti. NOTA: i tempi di asciugatura possono variare a seconda del design delle parti
e delle condizioni ambientali. Non lasciare le parti immerse nell’alcool isopropilico più a lungodel necessario.
2. Ispeziona le parti stampate per assicurarti che siano pulite e asciutte. Prima di passare alle fasi
successive, accertati che sulla superficie non sia rimasto alcun residuo di solvente, resina liquidain eccesso o frammenti.
3. Se noti residui di solvente, lascia asciugare le parti più a lungo. Se noti residui di resina, lava
nuovamente le parti finché non saranno pulite e asciutte.

E. POLIMERIZZAZIONE POST-STAMPA
Posiziona le parti stampate in un’unità di polimerizzazione post-stampa convalidata da Formlabs ed
esegui la polimerizzazione per il tempo richiesto.
1. Form Cure o Form Cure L:
a. Polimerizza per 60 minuti a 60 °C.
b. Lascia che l’unità Form Cure o Form Cure L si raffreddi fino a temperatura ambiente tra un ciclo
di polimerizzazione e il successivo.
2. Fast Cure:a. Polimerizza per sei minuti con intensità luminosa pari a 5.
b. Lascia raffreddare l’unità Fast Cure per almeno dieci minuti tra un ciclo di polimerizzazione
e il successivo.

F. RIMOZIONE DEI SUPPORTI E LUCIDATURA
1. Rimuovi i supporti utilizzando una tronchesina, un disco da taglio e un manipolo, o ricorrendo
ad altri strumenti di rimozione. Se sono evidenti segni irregolari sulla superficie delle parti dopo
la rimozione dei supporti, lucida/leviga questi punti per migliorare la finitura superficiale.
2. Ispeziona le parti per individuare eventuali crepe. Scarta le parti se rilevi danni o crepe.

G. PULIZIA E DISINFEZIONE
1. Le parti possono essere pulite, disinfettate e sterilizzate secondo i protocolli dell’impianto. A seguitodella disinfezione e/o sterilizzazione, è responsabilità dell’azienda produttrice convalidare leprestazioni delle parti in rapporto ai requisiti dell’applicazione. NOTA: se vengono utilizzati
disinfettanti a base di alcool, non lasciare le parti nella soluzione alcolica per un tempo prolungato.
2. Dopo la pulizia e la disinfezione, ispeziona la parte per verificare la presenza di eventuali danni ocrepe e assicurarti che l’integrità della parte progettata soddisfi i requisiti di prestazione. Scarta leparti se rilevi danni o crepe.

H. PERICOLI, CONSERVAZIONE E SMALTIMENTO
1. La resina polimerizzata non è pericolosa e può essere smaltita come un rifiuto comune.
2. Per ulteriori informazioni, consulta la scheda dati di sicurezza all’indirizzo support.formlabs.com.

Consideraciones específicas de fabricación
Las especificaciones de la BioMed White Resin se han validado utilizando el hardware y los parámetros
indicados a continuación. Para verificar la biocompatibilidad de la resina, el proceso de validación
utilizó un tanque de resina, un mezclador, una base de impresión, una unidad de lavado y equipamientode posacabado dedicados expresamente al material, que no se mezclaron con ninguna otra resina.

1. Hardware:a. Impresora 3D de Formlabs: Form 2, Form 3B/3B+, Form 3BL, Form 4B
b. Accesorios de impresión: Bases de impresión de Formlabs, tanques de resina de Formlabs

2. Software:a. PreForm de Formlabs

3. Parámetros de impresión:a. Grosor de capa: 100 μm y 50 μm

4. Equipamiento y accesorios recomendados para el posacabado:a. Accesorios de procesamiento de Formlabs: Form Auto, Resin Pumping Systemb. Unidad de lavado validada por Formlabs: Form Wash, Form Wash (2.ª generación), Form Wash L,
unidad de limpieza ultrasónica
c. Unidad de curado validada por Formlabs: Form Cure, Form Cure L, Fast Cure

A. IMPRESIÓN
1. Agitado del cartucho: Agita el cartucho antes de cada trabajo de impresión. Pueden darse
divergencias en el color y fallos de impresión si no se agita el cartucho lo suficiente.
2. Preparación: Inserta el cartucho de resina en una impresora 3D compatible de Formlabs.
Introduce el tanque de resina y acopla el mezclador al tanque.
3. Impresión:a. Prepara una impresión utilizando el software PreForm. Importa el archivo STL de la pieza deseada.
b. Orienta y genera los soportes.
c. Envía tu proyecto a la impresora.
d. Inicia la impresión seleccionando un proyecto en el menú de impresión. Sigue las instrucciones
o los diálogos que aparezcan en la pantalla de la impresora. La impresora completará
automáticamente la impresión.

B. EXTRACCIÓN DE LA PIEZA
Retira la base de impresión de la impresora. Para quitar las piezas de la base de impresión, coloca laherramienta para retirar piezas debajo de la base de la pieza impresa y gira la herramienta. Se puede
utilizar la Build Platform 2 o la Build Platform 2L de Formlabs para asegurar una extracción sencillay sin herramientas. Si deseas conocer las técnicas con detalle, visita support.formlabs.com.

C. LAVADO
Coloca las piezas impresas en una unidad de lavado validada por Formlabs con alcohol isopropílico
al 99 %.
1. Form Wash, Form Wash (2.ª generación) a alta velocidad* o Form Wash L:
a. Lava las piezas durante 5 minutos o hasta que estén limpias.
b. Si las piezas no parecen estar limpias después del lavado, considera reemplazar el alcohol
isopropílico usado de la unidad de lavado por disolvente nuevo.
*En el caso de la Form Wash (2ª generación), los ajustes de alta velocidad están validados para su uso.
2. Unidad de limpieza ultrasónica:ESPAÑOLLa BioMed White Resin es un material de resina fotocurable y polimerizable diseñado para la fabricación
aditiva de piezas médicas biocompatibles de color blanco, robustas y muy versátiles. Los usuarios
deberían verificar por su cuenta la idoneidad de los materiales impresos para su aplicación particular
y para el propósito previsto. Esta guía de fabricación ofrece recomendaciones y requisitos deequipamiento, impresión y posacabado para garantizar el uso correcto y seguro de este material.

NOTA: Utilizar alcohol isopropílico en un baño ultrasónico presenta un riesgo de incendio o explosión.
Cuando utilices un baño ultrasónico, lee y sigue todas las recomendaciones de seguridad delfabricante del baño ultrasónico.
a. Utiliza alcohol isopropílico al 99 % para cada limpieza.
b. Coloca las piezas en un recipiente de plástico desechable secundario o en una bolsa deplástico con cierre resellable y, a continuación, llénalo con alcohol isopropílico al 99 %,asegurándote de que las piezas queden totalmente sumergidas.
c. Coloca el recipiente secundario en el baño de agua de la unidad ultrasónica y somete laspiezas a ultrasonidos durante 2 minutos o hasta que estén limpias.**La eficacia del lavado depende del tamaño y la potencia de la unidad ultrasónica. Los ensayos
de Formlabs se realizaron con unidades ultrasónicas a 36 W/L o más.

D. SECADO
1. Saca las piezas del alcohol isopropílico y deja que se sequen al aire a temperatura ambiente
durante como mínimo 30 minutos. NOTA: Los tiempos de secado pueden variar según el diseño
de las piezas y las condiciones ambientales. No dejes las piezas en alcohol isopropílico mástiempo del necesario.
2. Inspecciona las piezas impresas para asegurarte de que estén limpias y secas. No deberían
quedar residuos de disolvente, resina líquida sobrante ni partículas residuales en la superficie
antes de pasar a pasos posteriores.
3. Si todavía queda disolvente residual, seca las piezas durante más tiempo. Si todavía hay residuos
de resina visibles, vuelve a lavar las piezas hasta que estén limpias y secas.

E. POSCURADO
Coloca las piezas impresas en una unidad de poscurado validada por Formlabs y cúralas durante eltiempo necesario.
1. Form Cure o Form Cure L:
a. Realiza un curado durante 60 minutos a 60 °C
b. Deja que la Form Cure o la Form Cure L se enfríe hasta la temperatura ambiente entre ciclos
de curado.
2. Fast Cure:a. Realiza un curado durante 6 minutos a intensidad de luz 5
b. Deja que la Fast Cure se enfríe durante al menos 10 minutos entre ciclos de curado.

F. RETIRADA Y PULIDO DE SOPORTES
1. Retira los soportes utilizando unos alicates de corte, un disco de corte y una herramienta de manou otras herramientas para retirar piezas impresas. Si es necesario, las partes ásperas que quedan
en la superficie de las piezas tras retirar los soportes se pueden pulir/lijar para mejorar el acabadode la superficie.
2. Inspecciona las piezas para comprobar que no tengan grietas. Desecha las piezas si detectas
daños o grietas.

G. LIMPIEZA Y DESINFECCIÓN
1. Las piezas se pueden limpiar, desinfectar y esterilizar de acuerdo con los protocolos del establecimiento.
Es responsabilidad del fabricante validar el rendimiento de la pieza en función de los requisitos de laaplicación tras la desinfección y/o esterilización. NOTA: Si se utilizan desinfectantes a base de alcohol,
no dejes las piezas en la solución alcohólica durante un tiempo prolongado.
2. Después de la limpieza y la desinfección, inspecciona la pieza para comprobar que no tiene
daños o grietas y que su integridad satisface los requisitos de rendimiento. Desecha las piezas si
detectas daños o grietas.

H. PELIGROS, ALMACENAMIENTO Y ELIMINACIÓN
1. La resina curada no es peligrosa y se puede desechar junto con los residuos habituales.
2. Si necesitas más información, consulta las FDS en support.formlabs.com.

특정 제조 고려 사항

BioMed 화이트 레진 사양은 아래에 표시된 하드웨어 및 매개변수를 사용하여 검증되었습니다. 생체적합성준수를 위해 다른 레진과 혼합되지 않도록 전용 레진 탱크와 믹서, 빌드 플랫폼, 세척 장치 및 후처리 장비를사용하여 검증을 진행했습니다.

1. 하드웨어:a. Formlabs 3D 프린터: Form 2, Form 3B/3B+, Form 3BL, Form 4B
b. 프린트 액세서리: Formlabs Build Platform, Formlabs Resin Tank

2. 소프트웨어:a. Formlabs PreForm

3. 프린팅 파라미터:a. 레이어 두께: 100㎛ 및 50㎛

4. 권장 후처리 장비 및 액세서리:a. Formlabs 가공 액세서리: Form Auto, Resin Pumping Systemb. Formlabs 검증 세척 장치: Form Wash, Form Wash(2세대), Form WashL, 초음파 세척 장치c. Formlabs의 검증된 경화 장치: Form Cure, Form Cure L, Fast CureA. 프린팅

1. 카트리지 혼합: 프린팅할 때마다 작업 전에 카트리지를 흔들어 주세요. 카트리지를 충분히 흔들지 않으면색상 편차가 발생하거나 프린팅에 실패할 수 있습니다.
2. 설정: 호환되는 Formlabs 3D 프린터에 레진 카트리지를 삽입합니다. 레진 탱크를 삽입하고 믹서를탱크에 부착합니다.
3. 프린팅:a. PreForm 소프트웨어를 사용하여 프린팅 작업을 준비합니다. 원하는 파트 STL 파일을 불러옵니다.
b. 방향 지정 및 서포트 생성c. 프린팅 작업을 프린터로 보냅니다.
d. 프린트 메뉴에서 프린트 작업을 선택하여 프린팅을 시작합니다. 프린터 화면에 표시되는 안내 메시지또는 대화 상자의 안내를 따릅니다. 프린터가 자동으로 프린팅을 완료합니다.

B. 파트 분리빌드 플렛폼을 프린터에서 꺼냅니다. 빌드 프랫폼에서 파트를 제거하려면 프린트된 파트 래프트 아래에 파트제거 도구를 끼워 넣은 후 도구를 회전시킵니다. Formlabs Build Platform 2 또는 Build Platform 2L을
사용하면 도구 없이 쉽게 제거할 수 있습니다. 자세한 기술은 support.formlabs.com을 참조하세요.

C. 세척프린트된 파트을 99% 이소프로필 알콜이 담긴 Formlabs의 검증을 거친 세척 장치에 넣습니다.
1. Form Wash, Form Wash(2세대) - 고속* 또는 Form Wash L:a. 5분간 또는 깨끗해질 때까지 세척합니다.
b. 세척 후 파트가 깨끗해 보이지 않으면 세척 장치에서 사용한 이소프로필 알코올을 새 것으로 교체하는것이 좋습니다.
*Form Wash (2세대)의 경우 고속 설정이 사용 가능한 것으로 확인되었습니다.
2. 초음파 세척 장치:
주의: 초음파 수조에서 이소프로필 알코올을 사용하면 화재나 폭발의 위험이 있습니다. 초음파 세척기를사용할 때는 초음파 세척기 제조업체의 안전 권장 사항을 빠짐 없이 읽고 따르세요.
a. 세척할 때마다 깨끗한 99% 이소프로필 알코올을 사용하세요.
b. 파트를 2차로 일회용 플라스틱 용기나 재밀봉 가능한 비닐 봉지에 넣은 다음 99% 이소프로필
알코올을 채워서 파트가 완전히 잠기도록 합니다.
c. 보조 용기를 초음파 장치 수조에 넣고 2분간 또는 깨끗해질 때까지 초음파 처리합니다*한국어

BioMed White Resin은 광경화성 중합성 수지 소재로, 견고하고 활용도가 매우 높은 생체 적합성 의료용백색 부품의 적층 제조에 사용됩니다. 프린트물이 특정 용도와 목적에 적합한지는 사용자가 개별적으로
확인해야 합니다. 본 제조 가이드에서는 이 자료의 정확하고 안전한 사용을 보장하기 위한 장비, 프린팅 및후처리 권장 사항과 요구 사항을 제공합니다.

*세척 효과는 초음파 장치의 크기와 출력 세기에 따라 달라집니다. Formlabs은 36W/L 이상의 초음파 장치로테스트를 수행했습니다.

D. 건조

1. 이소프로필 알코올에서 파트를 꺼내 실온에서 30분 이상 자연 건조시킵니다. 참고: 건조 시간은 파트의설계와 주변 조건에 따라 달라질 수 있습니다. 파트를 이소프로필 알코올에 필요 이상으로 오래 두지 마세요.
2. 프린팅된 파트를 검사하여 상태가 깨끗한지와 습기가 남아있지는 않은지 확인합니다. 다음 단계를진행하기 전에 표면에 잔류 용매, 과도한 액상 레진 또는 잔류 입자가 남아 있지 않아야 합니다.
3. 잔류 용제가 남아 있으면 파트를 더 오래 건조시키세요. 레진 잔여물이 여전히 보이면 깨끗하게 마를때까지 파트를 다시 세척합니다.

E. 후경화

프린트된 파트를 Formlabs의 검증을 거친 후 경화 장치에 넣고 필요한 시간 동안 경화합니다.
1. Form Cure 또는 Form Cure L
a. 60°C에서 60분간 경화b. 경화 사이클 사이에 Form Cure 또는 Form Cure L 장치를 실온까지 식힙니다.
2. Fast Curea. 광도 5에서 6분간 경화
b. Fast Cure 장치를 경화 주기 사이에 최소 10분 동안 식힙니다.

F. 서포트 제거 및 연마

1. 절단 플라이어, 절단 디스크 및 핸드피스를 사용하거나 다른 파트 분리 도구를 사용하여 서포트를제거합니다. 필요한 경우 서포트 제거 후 파트 표면에 남은 거친 자국은 표면 마감을 개선하기 위해 연마/샌딩하여 매끄럽게 처리할 수 있습니다.
2. 파트에 균열이 있는지 검사합니다. 손상이나 균열이 발견되면 폐기하십시오.

G. 청소 및 소독

1. 시설 프로토콜에 따라 부품을 세척, 소독 및 멸균할 수 있습니다. 제조업체는 소독 및/또는 멸균 후 적용요건에 따라 파트 성능을 검증할 책임이 있습니다. 참고: 알코올 기반 소독제를 사용하는 경우, 알코올용액에 파트를 장시간 방치하지 마세요.
2. 세척 및 소독 후 부품에 손상이나 균열이 있는지 검사하여 설계된 파트의 무결성이 성능 요구 사항을충족하는지 확인합니다. 손상이나 균열이 발견되면 폐기하십시오.

H. 위험, 보관 및 폐기

1. 경화된 레진은 위험하지 않으며 일반 폐기물로 처리할 수 있습니다.
2. 자세한 내용은 support.formlabs.com에서 SDS를 참조하세요.

製作に使用する際の留意事項

BioMed Whiteレジンの仕様に関しては、以下に示すハードウェアとパラメータを使用して検証を行っています。
生体適合性関連の基準に準拠し、他のレジンとの混合のない専用のレジンタンクとミキサー、
ビルド
プラットフォーム 、洗浄ユニット、後処理装置を使用して検証を行っています。

1. ハードウェア：

a. Formlabs 3Dプリンター：Form 2、Form 3B/3B+、Form 3BL、Form 4B
b. プリント用周辺機器：Formlabsビルドプラットフォーム、Formlabsレジンタンク

2. ソフトウェア：

a. Formlabs PreForm

3. プリントパラメータ：

a. 積層ピッチ：100 μm、50 μm

4. 推奨後処理装置と関連機器：

a. Formlabs製、後処理用装置：Form Auto、Resin Pumping Systemb. Formlabs検証済み洗浄ユニット：Form Wash、Form Wash（第2世代）、Form Wash L、超音波洗浄ユニット
c. Formlabs検証済み二次硬化ユニット：Form Cure、Form Cure L、Fast CureA. プリント手順

1. カートリッジを振る：プリントの都度、使用前にカートリッジをしっかり振ってください。
カートリッジの振り方が不十分な場合、色ムラが発生したり、プリントが失敗したりする原因になることがあります。
2. セットアップ：レジンカートリッジを互換性のあるFormlabs 3Dプリンターにセットします。
レジンタンクを挿入し、ミキサーをタンクに取り付けます。
3. プリント：a. PreFormソフトウェアを使用してプリントジョブを作成します。
プリントするSTLファイルをインポートします。
b. プリントの向きを決め、サポート材を生成します。
c. プリンターにプリントジョブを送信します。
d. プリントメニューに表示されるプリントジョブの中からジョブを選択し、プリントを開始します。
プリン
ターの画面に表示されるメッセージやダイアログに従って操作を進めます。
プリンターが自動的にプリントを完了します。

B. プリント品の取り外し

プリンターからビルドプラットフォーム を取り外します。
ビルドプラットフォームからプリント品を取り外すには、
リムーバルツールをプリント品のラフト下に差し込み、
リムーバルツールを回転させます。
Formlabs
Build Platform 2やBuild Platform 2Lを使用すれば、ツールなしで簡単に取り外すことが可能です。
詳細
手順は、support.formlabs.comをご覧ください。

C. 洗浄

99%イソプロピルアルコール（IPA）を入れたFormlabs検証済み洗浄ユニットに、プリント品を入れます。
1. Form Wash、Form Wash（第2世代）の高速洗浄*、またはForm Wash Lを使用する場合：
a. 5分間、またはきれいになるまで洗浄します。
b. 洗浄後、完全にきれいになっていない場合は、洗浄ユニット内の使用済みイソプロピルアルコールを新品と交換することをお勧めします。
*Form Wash（第2世代）を使用した高速洗浄は弊社検証済み。
2. 超音波洗浄ユニットを使用する場合：
注意：イソプロピルアルコールを超音波洗浄槽で使用すると、火災や爆発の危険がありますのでご注意く
ださい。
超音波洗浄機を使用する場合は、超音波洗浄機メーカーの推奨安全事項を読み従ってください。

日本語

BioMed White レジンは、生体適合性を備えた医療グレードの光硬化性（重合性）
レジン材料で、強度、汎用性に優れ、白色医療機器の積層造形向けに適しています。
本材料で製作した医療機器が、意図する使用や目的に適していることをご確認の上で使用してください。
本ガイドでは、
この材料を正しく安全に使用するための機器、
プリント手順、後処理に関する推奨事項や必要事項を説明しています。

a. 洗浄の都度、新しい99％イソプロピルアルコールを使用してください。
b. プリント品を、使い捨てのプラスチック容器またはジッパー付きのプラスチック袋に入れ、99％のイ
ソプロピルアルコールを入れて完全に浸漬します。
c. 別の容器を超音波ユニットの水槽に入れ、2分間、
またはきれいになるまで超音波処理を行います*。
*洗浄効果は、超音波ユニットのサイズと強度によって異なります。
Formlabsのテストは、36W/L以上の超音波ユニットで実施しています。

D. 乾燥

1. プリント品をイソプロピルアルコールから取り出し、室温で30分以上自然乾燥させます。
注記：乾燥時間は、プリント品の形状や周囲の環境によって異なる場合があります。
プリント品をイソプロピルアルコールに必要以上に長時間浸けないでください。
2. プリント品の全体を点検して、汚れがなく、きれいに乾いていることを確認します。
次のステップに進む
前に、溶剤や液体レジン、粉体が表面に残っていないことを確認してください。
3. 溶剤が残っている場合は、さらに乾燥させてください。
レジンが残っている場合は、
きれいになるまで再度洗浄した後、乾燥させてください。

E. 二次重合

プリント品をFormlabs認定品の二次重合ユニットに入れ、必要な時間重合させます。
1. Form CureまたはForm Cure L：
a. 60℃で 60分間硬化させます。
b. 次の硬化サイクルを実行する前に、Form CureまたはForm Cure Lユニットが室温まで冷めるのを待ちます。
2. Fast Cure：a. 光強度5で6分間硬化させます。
b. 次の硬化サイクルを実行する前に、Fast Cureユニットを10分以上放置して冷まします。

F. サポートの取り外しと研磨

1. カッティングプライヤー、
カッティングディスク、
ハンドピース、またはその他のリムーバルツール等を使って、サポート材を取り外します。
サポート材を取り除いた後の表面に粗い痕が残っている場合は、研磨用機
器やサンドペーパーで研磨してなめらかに仕上げます。
2. 仕上げ後、表面に亀裂などが発生していないかを確認します。
損傷や亀裂が見つかった場合は破棄してください。

G. 洗浄と消毒

1. 本レジンで製作した医療機器の洗浄、消毒、滅菌は、各医療機関の通例に従って行ってください。
製作した医療機器の消毒や滅菌後の性能の検証は、用途ごとの要件に基づき、製作を行った当事者の責任にて行ってください。
注記：アルコールベースの消毒剤を使用する場合は、プリントした機器をアルコール溶液に長時間放置しないでください。
2. 造形した医療機器の洗浄および消毒後、損傷や亀裂の有無を点検し、設計した医療機器が全体的に性能要件を満たしていることを確認します。
損傷や亀裂が見つかった場合は、破棄してください。

H. 危険性、保管、廃棄

1. 硬化したレジンは危険物ではないため、一般ごみとして廃棄可能です。
2. 詳細は、support.formlabs.comにある安全データシートをご覧ください。

具体生产注意事项

BioMed White Resin 规格已通过以下硬件和参数进行了验证。为了符合生物相容性要求，我们已使用专用的树脂槽和混合器、构建平台、清洗设备与后处理设备，在未与任何其他树脂混用的情况下进
行了验证。

1. 硬件：

a. Formlabs 3D 打印机：Form 2、Form 3B/3B+、Form 3BL、Form 4B
b. 打印配件：Formlabs 构建平台、Formlabs 树脂槽

2. 软件：

a. Formlabs PreForm

3. 打印参数：

a. 打印层厚：100μm 和 50μm

4. 建议使用的后处理设备和配件：

a. Formlabs 后处理配件：Form Auto（自动化系统）、Resin Pumping System（树脂泵送系统）b. 经 Formlabs 验证的清洗设备：Form Wash、Form Wash（第二代）、Form Wash L、超声波清洗装置
c. 经 Formlabs 验证的固化设备：Form Cure、Form Cure L、Fast Cure

A. 打印

1. 摇晃树脂盒：请在每次打印任务开始前摇晃树脂盒。如果未能充分摇晃树脂盒，可能会出现颜色偏差并造成打印失败。
2. 设置：将树脂盒放入兼容的 Formlabs 3D 打印机。插入树脂槽并将混合器安装到树脂槽中。
3. 打印：
a. 使用 PreForm 软件准备打印任务。导入所需的部件 STL 文件。
b. 定向并生成支撑结构。
c. 将打印任务发送至打印机。
d. 从打印菜单中选择打印任务以开始打印。请遵循打印机屏幕上的所有提示或对话框。打印机将自动完成打印。

B. 移除部件

从打印机中取出构建平台。如需从构建平台上移除部件，请将部件移除工具楔入打印部件基座下方，然后旋转工具。在不使用工具的情况下，用户可以从 Formlabs Build Platform 2 或 Build Platform 2L
上轻松移除部件。有关详细技术信息，请访问 support.formlabs.com。

C. 清洗

将打印好的部件放入经过 Formlabs 验证的装有 99% 异丙醇的清洗装置中。
1. Form Wash、Form Wash（第二代）－高速*，或 Form Wash L：
a. 清洗 5 分钟或直至洗净。
b. 如果部件在清洗后仍有脏污，请考虑使用纯净的溶剂替换清洗设备中使用过的异丙醇。
*Form Wash（第二代）的高速设置经验证可以使用。
2. 超声波清洗装置：
注：在超声波浴中使用异丙醇有发生火灾或爆炸的风险。在使用超声波清洗时，请阅读并遵守超声波清洗装置制造商的所有安全建议。
a. 每次清洗均需使用纯净的 99% 异丙醇。
b. 将部件放在辅助一次性塑料容器或可重新密封的塑料袋中，然后注入 99% 异丙醇，以确保完
全浸没部件。
c. 将辅助容器放在超声波装置的水浴中，超声处理 2 分钟或直至部件洁净。**清洗效果取决于超声波装置的大小和功率。Formlabs 采用了 36W/L 或更高的超声波装置进行测试。

中文

BioMed White Resin 是一种以光固化聚合物为原料的树脂，旨在通过增材制造技术制造具有生物相容性的医用级白色部件，使用这种材料打印的部件非常坚固，且用途极其广泛。使用者应独立验证该
打印材料是否适合其特定应用和预期用途。本制造指南中包含了设备、打印和后处理相关建议和要求，
可确保用户正确且安全地使用该材料。

D. 干燥

1. 从异丙醇中取出部件，并在室温下风干至少 30 分钟。注：干燥时间会因部件设计和环境条件而异。
请勿将部件在异丙醇中放置超过所需时间。
2. 检查打印部件，确保部件清洁干燥。确保部件表面无残留溶剂、多余的液态树脂或残余颗粒物，然后再进行后续步骤。
3. 如果仍然残留溶剂，则需延长部件干燥时间。如果仍存在可见的树脂残留物，请重新清洗部件，
直至清洁干燥。

E. 后固化

将打印部件放置于经 Formlabs 验证的后固化设备中，并按所需时间进行固化。
1. Form Cure 或 Form Cure L：
a. 在 60℃ 下固化 60 分钟
b. 每个固化周期结束后，请等待 Form Cure 或 Form Cure L 冷却至室温。
2. Fast Cure：a. 在光照强度 5 下固化 6 分钟b. 每个固化周期结束后，让 Fast Cure 冷却至少 10 分钟。

F. 支撑移除和抛光

1. 使用切割钳、切割盘和手持工具或使用其他后处理工具移除支撑。如果在移除支撑后部件表面残留
粗糙痕迹，可以视需要将其抛光/打磨光滑以改善表面光洁度。
2. 检查部件是否有裂痕。如果发现任何损坏或裂痕，则请将该部件丢弃。

G. 清洁和消毒

1. 可以根据设备规程对部件进行清洁、消毒和灭菌。完成消毒和/或灭菌后，制造商应负责根据应用要求验证部件性能。注：如果使用酒精类消毒剂，请勿将部件长时间浸泡在酒精溶液中。
2. 完成清洁和消毒后，检查打印部件是否损坏或存在裂缝，以确保设计的部件结构完整，可满足性能要求。如果发现任何损坏或裂痕，则请将该部件丢弃。

H. 危害、储存和处置

1. 固化树脂无害，可作为普通垃圾进行处置。
2. 请访问 support.formlabs.com 参阅安全数据表以获取更多信息。